Civil and Environmental Research ISSN 2224-5790 (Paper) ISSN 2225-0514 (Online) Vol.3, No.4, 2013 2.2.
Coconut fiber properties
The coconut fiber used in this study is derived waste coconut husk for industrial processing. Short coconut fibers were washed to remove dust and other impurities. The fibers were then dried at 30 째C for 24 h and filtered to separate the remaining impurities. The physical properties of the short fibers are as follow: length, 5 mm to 12.5 mm; diameter, 0.80-0.15 mm; and density, 600 kg/m3. Short coconut fibers after drying are as shown in Figure 2.
Figure 2. Micro-optic coconut fiber images 2.3.
Coconut fiber-asphalt (CFA) formulation
The coconut coir was cut to lengths of 5 mm, 7.5 mm, 10 mm, and 12.5 mm and added to the bitumen 60/70 in levels of 0.5%, 0.75%, 1%, 1.25%, and 1.5% by weight of asphalt. The fibers were added upon heating of the asphalt temperature to 150-160 째C by stirring for 5 min until the fibers were evenly mixed. Asphalt fiber can be stored and reheated when used for mixing with aggregate. Fiber size affects the ease of mixing between the asphalt and fiber: the smaller the fiber, the easier the mixing process. Coconut fiber will burn before the flash point of asphalt; thus, the mixing of the fibers and asphalt must be performed below the burning temperature of the coconut fibers. At the end of the test, the fibers were extracted from the bitumen to verify that the coconut fibers did not burn during the hot asphalt concrete mixing process. The results show that 96% coconut fiber mixed with bitumen remained after mixing. 2.4.
Mix design and optimization
The content of coconut fiber asphalt in the asphalt concrete mixture is equal to 6.36%. The asphalt was modified and the aggregate mixed at 155 째C. The samples were then brought to the compaction temperature of 10 째C less than the corresponding mixing temperature using a Marshall mechanical compactor. The specimens were compacted using 75 heavy-duty Marshall blows for each face, corresponding to a tire pressure of 1.379 kPa. Samples with a variety of fiber sizes and percentages of the asphalt were tested by Marshall, Marshall immersion, and wheel tracking tests. 3. 3.1.
Results and discussion Rheological tests
The CFA binder rheological properties were evaluated, and the results are presented in Table 4. The results show that the CFA is effective in improving the rheological properties of the asphalt cement. Table 4 reveals that the addition of CFA content reduces the penetration and ductility and increases the softening point. The results showed that the softening point of CFA modified increased by 2.3% and the penetration decreased by 11.5% with the addition of 0.75% coconut fiber (5 mm). The results also reveal that 0.75% CFA decreased the ductility to 47 cm, which shows that the CFA can still be used in asphalt cement. The increase in the softening point and decrease in the penetration can be attributed to the consistency of the CFA binder.